On the origin of emission and thermal quenching of SRSO:Er3+ films grown by ECR-PECVD
© Podhorodecki et al.; licensee Springer. 2013
Received: 8 October 2012
Accepted: 11 February 2013
Published: 22 February 2013
Silicon nanocrystals embedded in a silicon-rich silicon oxide matrix doped with Er3+ ions have been fabricated by electron cyclotron resonance plasma-enhanced chemical vapor deposition. Indirect excitation of erbium photoluminescence via silicon nanocrystals has been investigated. Temperature quenching of the photoluminescence originating from the silicon nanocrystals and the erbium ions has been observed. Activation energies of the thermally activated quenching process were estimated for different excitation wavelengths. The temperature quenching mechanism of the emission is discussed. Also, the origin of visible emission and kinetic properties of Er-related emission have been discussed in details.
Rare-earth-doped materials have been investigated for a number of years in order to develop practical light sources for photonic applications. A silicon-rich silicon oxide (SRSO) matrix seems to be very promising as an efficient photosensitizer for different rare-earth (RE) ions such as: Nd3+[1, 2], Tb3+, or Er3+[4, 5]. Among these ions, the Er3+ ion is well known as an alternative to epitaxially grown light sources emitting in the third telecommunication window [6, 7]. One of the advantages of a SRSO matrix as a host for RE ions is the formation of Si nanocrystals (Si-NCs) within the matrix which could participate in indirect excitation of Er3+ ions via an energy transfer process. Additionally, these clusters can improve the film’s conductivity, which in practice can be an even more important benefit. The advantage of using Si-NCs comes from their high absorption cross section (σabs) as compared to very low ones for most of the RE ions. For example, for erbium in SiO2, the experimentally determined value of σabs is 8 × 10-21 cm2, while for Si-NCs at 488 nm, this value is equal to 10-16 cm2. Moreover, Franzo et al.  and Gourbilleau et al. reported already that amorphous Si nanoclusters (a Si-NCs) can be sufficient and even better sensitizers than Si-NCs, enhancing the optical activity of Er3+ ions. Thus, enriching SiO2 with Si nanocrystals or amorphous nanoclusters should significantly increase Er3+ emission due to their indirect excitation. However, to date, achieving gain from this material has proven to be a notoriously difficult task. This is, in part, due to the low excitable Er3+ fraction sensitized through the Si-NCs (0.5% to 3% [12, 13]) and the low number of excitable Er3+ ions per nanocrystal (1 to 2 [14, 15] or 20 ), which affects the maximum gain that can be achieved in a Si-sensitized gain medium. It is believed that the low number of optically active Er3+ ions coupled to Si-NCs is due to processes like fast Auger back-transfer from excited Er3+ ions to excitons in Si-NCs, excited-state absorption, or Er3+ pair-induced quenching. Nevertheless, experimental data strengthening or excluding any of these explanations is still limited. One of the exceptions is recent work of Navarro-Urrios et al.  who have shown that none of these processes are responsible for the low fraction of Er3+ coupled to Si-NCs, and only the short range of interaction between Si-NCs and Er3+ (0.5 nm) is the main limitation to achieving a high fraction of ions coupled to Si-NCs. As a consequence, it has been shown that the amount of excitable Er3+ depends strongly on the Si-NC density as only those Er3+ ions in close proximity to the Si-NCs are being excited . Therefore, it is believed that the main limitation on obtaining gain in such a system is the low density of sensitizers, the short range of the Si-NCs and Er3+ interaction , and low solubility of Er3+ ions in SRSO matrix.
However, in addition to weak Si-NCs-Er3+ coupling, reduction in Er3+ emission efficiency can also be due to many quenching processes accompanying the excitation and recombination of Er3+ ions. Such processes still have not been widely investigated. Furthermore, even today, the detailed excitation mechanism of Er3+ ions in SRSO is still not well understood. Investigations of time-resolved photoluminescence of Er3+ ions in SRSO reveal two major excitation mechanisms leading to 1.5-μm emission, distinguishable by their dynamics: a fast relaxation within the Si-NCs and energy transfer to ions (<100 ns), taking Er3+ ions directly to the first excited state, and a slow relaxation and energy transfer, exciting Er3+ ions to higher states. In both cases, however, the emission decay should be slowed down due to slow radiative relaxation from 4I13/ 2 to 4I15/ 2 on a millisecond-microsecond time scale [18–20]. The fast energy transfer has already been related to Auger-type excitation of Er3+ ions directly from the Si-NCs to 4I13/ 2 level of Er3+ ions. In this case, excited ions should be inside the core of Si-NCs or at their surface due to the short range of Auger-type interactions. This mechanism can also be discussed since to obtain a high efficiency of Auger recombination within the Si-NCs, the energy levels of Si-NCs should be well separated from each other to minimize thermal relaxation which strongly reduces the Auger-type relaxation. It has been shown, however, theoretically that for Si-NCs, especially when surface/matrix interface is included into the calculations, the energy spectrum of Si-NCs is almost continuous above the main absorption edge [21, 22]. Besides, it has been shown recently that in the spectral range of Er3+ emission, another emission with nanosecond decay appears which, however, cannot be related to Er3+ ions. This emission can be assigned more likely to defect states in the SRSO film. Thus, many open questions regarding the origin of the fast process still remain.
It is widely believed that the slow process is due to dipole-dipole energy transfer either from the exciton confined inside the Si-NCs or localized at their surface states. In this case, the transfer can occur efficiently (with a rate of 109 s-1) to the ions located even 6 to 7 nm from the Si-NCs, as has been shown by Choy et al. . On the contrary, other authors have proposed that the optimal distance between Si-NCs and Er3+ ions is on the order of 0.5 nm only [24, 25]. With such a short interaction distance, the question regarding the nature of energy transfer and validity of dipole-dipole interaction only became important. Moreover, in case of slow energy transfer, the intermediate defect states in the SRSO matrix became important and can also participate in Er3+ excitation allowing exciton migration before the exciton transfers its energy to Er3+ ions. This should also increase the distance of Si-NC-Er3+ interaction. In view of the above discussion, understanding of the origin of visible emission and temperature quenching of the emission of Er3+ becomes important to understand the efficiency of coupling between Er3+ and Si-NCs as well as the energy transfer between them.
There are several processes which might be responsible for temperature quenching of the photoluminescence (PL) in Si-NCs, such as (a) carriers’ resonant/non-resonant tunneling out of Si-NCs to sites where the non-radiative recombination occurs , (b) thermal activation of carriers over the potential barrier Si/SiO2 (3.4 eV) , and (c) simply non-radiative band-to-band transition. Other potential mechanisms, such as exciton dissociation (approximately 14 meV for bulk Si ) should rather be excluded from consideration in the case of Si-NCs since within the Si-NCs, there are no excitonic levels other than the ones related to Si-NCs itself, where the Columbic interaction has been included in self-consistent calculations. Thus, there are no additional levels to which the exciton could dissociate as in the case of bulk material. The only quenching energy which could be associated with exciton dissociation is one which moves one of the carriers to defect levels at the surface of Si-NCs over the potential barrier (process a or b). The only temperature-dependent emission-quenching mechanisms related to the excitonic nature of carriers confined within the Si-NCs can be due to different spin selection rules for different energy levels, which give the dark and bright states, which can be split in Si-NCs even with 20 meV .
In the case of erbium ions, PL quenching can be related to back-transfer mechanisms , which should be, however, very inefficient in Si-NCs because of the large difference in Er3+ emission energy and the absorption edge of Si-NCs . Another common mechanism responsible for the quenching of PL originating from Er3+ is Auger recombination between excited Er3+ and excess electrons bound to a surface/defect state at Si-NCs . Finally, Er3+ can transfer energy due to dipole-dipole interactions to other ions or to defect states which play the role of quenching centers. In order to be temperature-dependent, all these quenching processes should be phonon assisted.
In view of the above discussion, it can be seen that even if work on SRSO: Er3+-based LEDs is already advanced  from the fundamental point of view, there are many uncertainties and contradicting results in the literature. We believe that one of the main reasons is simplification of the interpretation of the obtained emission signal as related to Si-NCs only and the unappreciated role of the complex nature of the SRSO film where defects and both a Si-NCs and Si-NCs can be optically active simultaneously in the same spectral range. Moreover, in many cases, the 488-nm line is used for SRSO:Er3+ excitation, where this wavelength overlaps with one of the optical transitions of Er3+ ions and can bring about interpretation of obtained data.
In this work, we present new data regarding excitation, recombination, and thermal quenching of Er3+-related emission. As the absorption cross sections of Si-NCs and Er3+ ions are different by orders of magnitude, the excitation of Er3+ via Si-NCs at low excitation power should dominate over their direct excitation. Thus, as an additional aim of this work, we examine the optical properties of SRSO:Er3+ at an excitation truly resonant with 4f-4f energy levels (980 nm), at indirect excitation (266 nm), and at 488-nm excitation wavelength, the non-resonant nature of which is questionable.
The Er-doped SRSO film was grown on a Si substrate by electron cyclotron resonance plasma-enhanced chemical vapor deposition (ECR-PECVD) using SiH4 and O2 source gases diluted in Ar to form the SRSO matrix. Er(TMHD)3 was employed as the rare-earth precursor to achieve high concentrations of Er doping. The film was annealed in a quartz tube furnace under flowing ultrahigh-purity N2 for 1 h. The annealing temperature was 1,100°C. As we have shown in many previous papers, in our deposition system, this temperature is sufficient to obtain silicon nanocrystals of a few nanometers in size, both in the absence of erbium doping  and in the case of doping with erbium and different lanthanides [33, 34]. The deposition system has been described in detail elsewhere . The composition of the film (39 and 37 at.% of Si and 0.45 at.% of Er) was measured by Rutherford backscattering spectrometry. The film thickness estimated from ellipsometry experiments was 200 nm for both samples.
The room-temperature photoluminescence excitation (PLE) of the erbium ions in the near-infrared (NIR) was measured using an InGaAs pin photodiode. As an excitation source, a 450-W Xe arc lamp connected to a Triax 180 monochromator (Jobin-Yvon, Kyoto, Japan) was used. PL as a function of temperature was excited using a 488-nm Ar+ CW laser (Melles Griot, Albuquerque, NW, USA), 266-nm (Elforlight, Daventry, UK) and 980-nm (Opolette™, Opotek Inc., Carlsbad, CA, USA) pulse lasers. An HR4000 spectrometer (Ocean Optics, Dunedin, FL, USA) and InGaAs CCD linear detector (Symphony® I line, Horiba Jobin-Yvon) were used as detection systems for measurements in the visible (VIS) and NIR spectral range, respectively. The PL decay was measured using pulsed laser coupled to a gated detection system (QuantaMaster from Photon Technology International, London, Canada).
Results and discussion
The second band at 1.6 eV can be assigned to the recombination of excitons localized in the SRSO matrix. Moreover, from Figure 1a, it can be seen that all VIS emission bands have a complex structure. This is due to interference effects caused by the refractive index contrast between SRSO and the Si substrate . These interferences will modify the shape of the emission spectra in the entire VIS spectral range. However, Er3+ emission is not affected by this effect.
Additionally, Figure 1a shows the PLE spectra measured for Er3+ at room temperature at 0.81 eV in a broad UV-VIS excitation band energy range. The obtained PLE spectra are also very similar to those obtained by us for undoped SRSO samples [36, 37]. The appearance of strong Er3+ emission at excitation wavelengths far from resonance with erbium energy levels clearly indicates that we are dealing here with an efficient excitation transfer from the levels responsible for VIS emission (i.e., a Si-NCs, Si-NCs, or defects) to erbium ions. The main argument behind the conclusion that defect states can be excluded in this case is the Si-concentration-dependent position of the excitation spectra for Er3+ ions and VIS emission bands. It can be seen that when the Si content increases, the edge of excitation as well as emission bands shifts towards lower energies due to reduction of quantum confinement. This suggests that the observed VIS emission can be related either to a Si-NCs or to Si-NCs. Moreover, the position of these excitation bands at 4.3 and 3.4 eV for 37 and 39 at.% of Si, respectively, seems to be different than energies typically obtained for excitation bands of defects in SiO2 films: ‘non-bridging oxygen hole center’ at 4.8 and 5.8 eV , E’ center at 5.4 to 6.2 eV , or ‘oxygen-deficient center’ (ODC) at 7.6, 6.9, and 5.0 eV .
where f(E) is the Fermi probability function defined as f(E) = [1 + exp(E - E F /kT)]-1, where k is Boltzmann’s constant and T is the ambient temperature. Thus, at a low temperature, carriers relax to the lowest levels within the tails of LDOS. However, when the temperature increases, carriers move to higher lying levels and recombine at higher energies. Moreover, due to the increased role of non-radiative channels at a high temperature, the emission decay time is reduced, and thus, carriers can recombine from higher levels, also moving the emission band towards higher energies. Thus, the observed emission band at 1.6 eV can be related mainly to a Si-NCs. However, we cannot exclude additional contributions to the observed emission from Si-NCs.
From Figure 1, we can clearly see the redshift of the total VIS emission with increasing Si content. Based on the above results, the observed shift can be explained as due to changes in a Si-NC sizes (redshift due to quantum confinement effect), changes in number of defect states making contributions to tails of LDOS (blue- or redshift), relative contribution of emission bands from matrix-related defect states, or Si-NC- and a Si-NC-related emission. Moreover, increasing strain at the Si-NCs/SiO2 interface with Si atomic percent should also be included as it has been shown by us recently elsewhere . This can introduce defect states and can also influence the position of the energy levels related to Si-NCs inducing both red- and blueshift.
Based on the results obtained so far, we conclude that the observed wide emission band obtained usually at CW excitation is a superposition of three emission sub-bands coming from spatially resolved objects with very different kinetics: (1) a band at around 450 nm, with 20-ns decay, which is not changing its position with Si content and is related to optically active defect states and STE in the SRSO matrix; (2) a band at around 600 nm related to a Si-NCs with hundreds of microsecond emission decay and strong dependence on Si content following the predictions of the quantum confinement model; (3) and a third band at around 800 nm (1.54 eV) (Si-NCs, defects) with either very fast (<3 ns) or very slow (>100 μs) emission kinetics also depending on Si content. In this case, however, an increase in Si content influences only the relative intensities between this band and the a Si-NC emission bands. This band can be related to Si-NCs or defect-related states. The weak dependence of the position of this band on Si content can be due to the weak quantum confinement regime. Based on our previous XRD and Raman results for similar samples, we can assume that the size of Si-NCs is in the range of 4 to 6 nm.
In summary, two components often obtained in emission decay times when the signal is recorded at one energy can be due to different spatially resolved objects (a Si-NCs and Si-NCs or defects) rather than two relaxation mechanisms different in timescale related with one object only, i.e., Si-NCs or a Si-NCs. The second conclusion that can be given based on the obtained preliminary results is that in many cases, the shift of the emission band at CW excitation observed for samples either annealed at different temperatures or obtained at different excess Si contents can be due to different contributions of defect states into this band. This shift is often related to changes in Si-NC size only. However, at the same time, these two technological parameters change also the number of defects in the matrix, induce a phase transition of Si clusters from amorphous to crystalline, influence the lanthanide distribution , and modify the strain at the clusters’ interface, increasing/reducing the tails of density of states .
where α(τ) is the recovered distribution and m(τ) is the assumed starting distribution. In this equation, τ = 1/k, and the relation between g(k) and α(τ) is α(τ) = τ-2g(1/τ). MEM allows finding α(τ) without any previous knowledge that we may have about the rate distribution. This method has been successfully applied in many situations where the inverse problem is highly degenerate, owing to the presence of noise in the data or the large parameter space one is working with.
Thus, based on the above approach, we fit our data with two exponential functions. It should be mentioned that an important aspect of MEM is that even purely exponential decay processes have decay time distributions with finite width (unless the data is completely noiseless). Therefore, the broad distributions obtained by MEM, i.e., in the case of 488-nm excitation for 37 at.% of Si sample, do not necessarily imply non-exponential dynamics. A test to verify this is to fit the data with exponential decays taking the peaks of the distributions as the decay times. In the investigated case, the PL decay can be fitted very well with a two-exponential decay (χ2 ≈ 1.0), yielding decay times of 4,860 and 885 μs and 2,830 and 360 μs for the samples with 37 and 39 at.% of Si, respectively. The obtained decay times are almost the same as the distribution peaks shown in Figure 3. This result allows us to conclude that the PL decay for both samples can be described by two exponential functions. It should be emphasized that this conclusion could not be drawn without MEM analysis since the PL decays can be fit well also with other models, e.g., the stretched exponential function of the form I(t) ~ tβ-1∙exp(-(t/τ)β). However, in the case of the stretched exponential function, the distribution α(τ) should exhibit the power-law asymptotic behavior of the form α(τ) ~ tβ-1, for t → 0, which is not the case.
Thus, at 266-nm excitation for both samples, we obtained emission decay times characterized by two components: a fast one (<1 ms) and a slow one (approximately 3 ms). Since the radiative transitions in Er3+ are only weakly allowed, the cross sections for optical excitation and stimulated emission are quite small, typically in the order of 10-21 cm2. Because of that, the radiative lifetime of the 4I13/2 → 4I15/2 transition in Er3+ ions excited directly in SRSO should lie between 14 ms for pure silica  and 1 ms for silicon .
The longer time obtained by us is typical for times obtained by other authors (i.e., SiO, 2.5 to 3.5 ms  and SRSO, 2 to 11 ms [11, 50–52]). To explain the second component of our samples, we have three options: (a) Er3+ ions are excited via a Si/Si-NCs, and there is only one optically active Er3+ site excited by two temporally different mechanisms; (b) Er3+ ions are excited via a Si/Si-NCs, and there are two different Er3+ sites, i.e., the isolated ion and clusters of ions; and (c) optically active Er3+ ions are excited via Si-NCs and a Si-NCs or defect states separately with a different kinetics .
Nevertheless, even if the above models could explain two different times recorded for Er3+ emission, the short time observed for Er3+ seems to be much shorter than expected. This could be explained only by the assumption that the short emission decay can be related to Er3+ ions which interact with each other, and due to ion-ion interaction, their emission time can be significantly reduced. Efficient clustering of lanthanides and especially Er3+ ions has already been shown by us and other authors [3, 25]. Thus, we propose that the slow component is due to emission from isolated ions, while the fast component is related with the ions in a cluster form.
where n is the refractive index of the matrix, <ΨJ′| and |ΨJ> are the initial and final states of single parity, U(λ) is the irreducible tensor form of the dipole operator, λ is the emission wavelength, and Ωλ are the Judd-Ofelt parameters, describing the local environment of the ion. We have observed similar effects of the influence of n on the emission decay time recently for Tb3+ ions introduced into a SRSO matrix where the Si concentration was changed from 35% to 40%, increasing the refractive index from 1.55 to 1.70. Additionally, this reduction in decay time can be also due to an increased number of non-radiative channels with increasing Si content making contributions to the final emission decay as τPL-1 = τR-1 + τNR-1. Similar results have been obtained when 488 nm was used as the excitation wavelength. Moreover, reduction in emission decay time has been observed when the excitation wavelength is changed. The emission decay time at 488 and 266 nm can be different when two different sites are excited at different wavelengths. To verify this, emission spectra of Er3+ ions obtained at 10 K have been compared at different excitation wavelengths. In the limit of our system resolution, we did not find any difference in the emission peak position at different excitation wavelengths. Thus, we believe that the same sites emit at 1,535 nm at all excitation wavelengths.
To investigate the effect of emission quenching, we have performed PL measurements as a function of temperature for different excitation wavelengths. In order to interpret these results, we considered the temperature dependence of the PL intensity at low pump power according to the Arrhenius law with EQ as deactivation (ionization) energy.
Based on the FTIR and Raman spectroscopy done on our samples previously , we found several absorption bands related with phonons or SRSO matrix vibrations which can participate in thermal quenching. Typical Raman spectra obtained by us for these samples consist of two bands: a broad low-frequency band (LF) with maximum at around 485 cm-1 (59 meV) and a narrower, asymmetrically broadened high-frequency (HF) peak centered at 520 cm-1(64 meV). The LF band may be attributed to a Si present in the matrix, whereas the HF originates from Si-NCs. Moreover, from the FTIR spectra, there are three main bands located at 1,000 to 1,300 cm-1 (123 to 161 meV) and 800 cm-1 (100 meV) related to the asymmetric stretching and bending Si-O-Si modes, respectively.
In general, the quenching of the luminescence with temperature can be explained by thermal emission of the carriers out of a confining potential with an activation energy correlated with the depth of the confining potential. Since the observed activation energy is much less than the band offsets between Si/SiO2 (approximately 3.4 eV), the thermal quenching of the a Si/Si-NC-related emission is not due to the simple thermal activation of electrons and/or holes from the a Si/Si-NCs potential into the SiO2 barriers. Instead, the dominant mechanism leading to the quenching of the VIS-related PL is due to the phonon-assisted tunneling  of confined carriers to states at the interface between a Si/Si-NCs and the matrix.
Analyzing the data presented in Figure 4a,d, we can see that when the Er3+ is excited with 266 nm, PL thermal quenching can be well fitted only when two quenching energies are used. For both samples, these energies are equal to EErQ1 ~ 15 meV and EErQ2 ~ 50 meV. For comparison, in Figure 4a,d, two fits have been shown with one and two quenching energies. It is clear that two energies are needed to obtain a statistically good fit. Once we look at thermal quenching recorded for the emission related to a Si/Si-NCs, we can see that the thermal quenching can also be fitted with two energies similar for both samples: EVISQ1 ~ 10 and EVISQ2 ~ 65 meV.
The EVISQ2 energy corresponds exactly to the energy of phonons related to oscillations of Si-Si bonds obtained in Raman experiments. In more detail, this value is closer to the amorphous phase of silicon rather than the crystalline phase. This could be related to the fact that amorphous nanoclusters are responsible for the observed emission in the VIS range as well as for the indirect excitation of Er3+ ions. Thus, most probably at a temperature corresponding to 65 meV, one of the carriers is moved from the potential related with a Si-NCs to defects states at their surface, where it recombines non-radiatively or diffuses over longer distances inside the matrix. The second energy (EVISQ1) is much less clear at the moment. Nevertheless, correlation between the second quenching energy (55 meV) observed for Er3+ emission with the quenching energy obtained for a Si-NC emission (65 meV) suggests efficient coupling between these two objects and confirms that most of the quenching appears before the excitation energy is transferred from a Si-NCs to Er3+ ions. Also, at this excitation, Er3+-related emission is quenched by factors of 6 and 11 for samples with 37 and 39 at.% of Si, respectively.
Figure 4e shows results of thermal emission quenching at 488-nm excitation wavelength for a sample with 39 at.% of Si. It can be seen that the Er3+-related emission is also characterized by two quenching energies equal to about 20 and 60 meV. These values are almost the same as for 266-nm excitation and very similar to VIS emission where values of 15 and 70 meV have been obtained. This indicates that in this case also, we deal with indirect excitation of Er3+ ions. Since 488 nm corresponds also to direct excitation of Er3+ ions, most probably, we deal with both kinds of excitation simultaneously. We believe, however, that indirect excitation is in this case dominant. Nevertheless, the results obtained at this excitation wavelength for 37 at.% of Si are not so obvious. In this case, two statistically equal fits with one (20 meV) and two energies (20 and 6 meV) were possible to achieve. The higher energy is clear and has the same origin as in the previous cases. One explanation of this fact would be the excitation spectrum for this sample where its edge is much shifted to blue as compared to samples with 39 at.% of Si. Thus, in this case, we can indeed observe a major contribution from a direct excitation of Er3+ ions rather than via intermediate states.
The existence of efficient excitation transfer from silicon nanoclusters to Er3+ ions has been shown for SRSO thin films deposited by ECR-PECVD by means of PL, TRPL, PLE and temperature-dependent PL experiments. However, it has been shown that for our samples, this energy transfer is most efficient at high excitation energies. Much less efficient energy transfer has been observed at 488-nm excitation. In this case, depending on Si nanocluster size, we deal with dominant contribution to Er3+ excitation from indirect excitation channel (big nanoclusters) or from direct excitation of Er3+ ions (small nanoclusters).
Moreover, it has been shown that a wide emission band in the VIS spectral range is a superposition of three emission sub-bands coming from spatially resolved objects with very different kinetics: a band at around 450 nm, with 20-ns decay, which is not changing with Si content and is related with optically active defect states and STE in SRSO matrix; a band at approximately 600 nm related to a Si-NCs with hundred-microsecond emission decay and strong dependence on Si content following the predictions of quantum confinement model; and a third band at around 800 nm (1.54 eV) (Si-NCs, defects) with either very fast (<3 ns) or very slow (>100 μs) emission kinetics, also depending on Si content. Additionally, it has been shown that two Er3+ sites are present in our samples: isolated ions and clustered ions with emission decay times of approximately 3 and <1 ms, respectively.
AP would like to acknowledge the financial support from the Iuventus Plus program (no. IP2011 042971). In Canada, the work was supported by the Natural Sciences and Engineering Research Council of Canada under the Discovery Grants Program.
- Podhorodecki A, Misiewicz J, Gourbilleau F, Dufour C: Direct evidence of the energy transfer from silicon nanocrystals to Nd ions. Electrochemical Solid State Lett 2010, 13: K26-K28. 10.1149/1.3279688View Article
- Watanabe K, Tamaoka H, Fujii M, Moriwaki K, Hayashi S: Excitation of Nd3+ and Tm3+ by energy transfer from Si nanocrystals. Physica E 2002, 13: 1038–1042. 10.1016/S1386-9477(02)00297-7View Article
- Podhorodecki A, Zatryb G, Misiewicz J, Wojcik J, Wilson PRJ, Mascher P: Green light emission from terbium doped silicon rich silicon oxide films obtained by plasma enhanced chemical vapor deposition. Nanotechnology 2012, 23: 475707. 10.1088/0957-4484/23/47/475707View Article
- Shin JH, Seo SY, Kim S, Bishop SG: Photoluminescence excitation spectroscopy of erbium-doped silicon-rich silicon oxide. Appl Phys Lett 1999, 2000: 76.
- Khomenkova L, Gourbilleau F, Cardin J, Jambois O, Garrido B, Rizk R: Long lifetime and efficient emission from Er3+ ions coupled to Si nanoclusters in Si-rich SiO2 layers. J Lum 2009, 129: 1519–1523. 10.1016/j.jlumin.2009.01.030View Article
- Podhorodecki A, Andrzejewski A, Kudrawiec R, Misiewicz J, Wojcik J, Robinson BJ, Roschuk T, Thompson DA, Mascher P: Photoreflectance investigations of quantum well intermixing processes in compressively strained InGaAsP/InGaAsP QW laser structures emitting at 1.55 μm. J App Phys 2006, 100: 013111–1-013111–12.View Article
- Ramirez JM, Lupi FF, Jambois O, Berencen Y, Navarro-Urrios D, Anopchenko A, Marconi A, Prtljaga N, Tengattini A, Pavesi L, Colonna JP, Fedeli JM, Garrido B: Erbium emission in MOS light emitting devices: from energy transfer to direct impact excitation. Nanotechnology 2012, 23: 125203. 10.1088/0957-4484/23/12/125203View Article
- Takahei K, Taguchi A: Energy transfer in rare-earth-doped III-V semiconductors. Mater Sci Forum 1992, 83–87: 641–652.View Article
- Priolo F, Franzò G, Pacifici D, Vinciguerra V, Iacona F, Irrera A: Role of the energy transfer in the optical properties of undoped and Er-doped interacting Si nanocrystals. J Appl Phys 2001, 89: 264. 10.1063/1.1331074View Article
- Franzo G, Boninelli S, Pacifici D, Priolo F, Iacona F, Bongiorno C: Sensitizing properties of amorphous Si clusters on the 1.54-μm luminescence of Er in Si-rich SiO2. Appl Phys Lett 2003, 82: 3871. 10.1063/1.1579555View Article
- Gourbilleau F, Levalois M, Dufour C, Vicens J, Rizk R: Optimized conditions for an enhanced coupling rate between Er ions and Si nanoclusters for an improved 1.54-μm emission. J Appl Phys 2004, 95: 3717. 10.1063/1.1655680View Article
- Wojdak M, Klik M, Forcales M, Gusev OB, Gregorkiewicz T, Pacifici D, Franzò G, Priolo F, Iacona F: Sensitization of Er luminescence by Si nanoclusters. Phys Rev B 2004, 69: 233315.View Article
- Garrido B, Garcia C, Seo SY, Pellegrino P, Navarro-Urrios D, Daldosso N, Pavesi L, Gourbilleau F, Rizk R: Excitable Er fraction and quenching phenomena in Er-doped SiO2 layers containing Si nanoclusters. Phys Rev B 2007, 76: 245308.View Article
- Kik PG, Polman A: Exciton–erbium interactions in Si nanocrystal-doped SiO2. J Appl Phys 1992, 2000: 88.
- Kik PG, Polman A: Gain limiting processes in Er-doped Si nanocrystal waveguides in SiO2. J Appl Phys 2002, 91: 534. 10.1063/1.1418417View Article
- Navarro-Urrios D, Pitanti A, Daldosso N, Gourbilleau F, Rizk R, Garrido B, Pavesi L: Energy transfer between amorphous Si nanoclusters and Er3+ ions in SiO2 matrix. Phys Rev B 2009, 79: 193312.View Article
- Garcia C, Pellegrino P, Lebour Y, Garrido B, Gourbilleau F, Rizk R: Maximum fraction of Er3+ ions optically pumped through Si nanoclusters. J Lumin 2006, 121: 204–208. 10.1016/j.jlumin.2006.07.026View Article
- Fujii F, Imakita K, Watanabe K, Hayashi S: Coexistence of two different energy transfer processes in SiO2 films containing Si nanocrystals and Er. J Appl Phys 2004, 95: 272. 10.1063/1.1631072View Article
- Savchyn O, Todi RM, Coffey KR, Kik PG: Observation of temperature-independent internal Er3+ relaxation efficiency in Si-rich SiO2 films. Appl Phys Lett 2009, 4: 241115.View Article
- Izeddin I, Moskalenko AS, Yassievich IN, Fujii M, Gregorkiewicz T: Nanosecond dynamics of the near-infrared photoluminescence of Er-Doped SiO2 sensitized with Si nanocrystals. Phys Rev Lett 2006, 97: 207401.View Article
- Seino K, Bechstedt F, Kroll P: Influence of SiO2 matrix on electronic and optical properties of Si nanocrystals. Nanotechnology 2009, 20: 135702. 10.1088/0957-4484/20/13/135702View Article
- Guerra R, Marri I, Magri R, Martin-Samos L, Pulci O, Degoli E, Ossicini S: Silicon nanocrystallites in a SiO2 matrix: role of disorder and size. Phys Rev B 2009, 79: 155320.View Article
- Choy K, Lenz F, Liang XX, Marsiglio F, Meldrum A: Geometrical effects in the energy transfer mechanism for silicon nanocrystals and Er3+. Appl Phys Lett 2008, 93: 261109. 10.1063/1.3058440View Article
- Gourbilleau F, Dufour C, Madelon R, Rizk R: Effects of Si nanocluster size and carrier–Er interaction distance on the efficiency of energy transfer. J Lumin 2007, 126: 581–589. 10.1016/j.jlumin.2006.10.008View Article
- Pellegrino P, Garrido B, Arbiol J, Garcia C, Lebour Y, Morante JR: Site of Er ions in silica layers codoped with Si nanoclusters and Er. Appl Phys Lett 2006, 88: 121915. 10.1063/1.2190267View Article
- Vial JC, Bsiesy A, Gaspard F, Herino R, Ligeon M, Muller F, Romestain R: Mechanisms of visible-light emission from electro-oxidized porous silicon. Phys Rev B 1992, 45: 14171. 10.1103/PhysRevB.45.14171View Article
- Suemoto T, Tanaka K, Nakajima A: Interpretation of the temperature dependence of the luminescence intensity, lifetime, and decay profiles in porous Si. Phys Rev B 1994, 49: 11005. 10.1103/PhysRevB.49.11005View Article
- Shaklee KL, Nahory RE: Valley-orbit splitting of free excitons? The absorption edge of Si. Phys Rev Lett 1970, 24: 942. 10.1103/PhysRevLett.24.942View Article
- Brongersma ML, Kik PG, Polman A, Min KS, Atwater HA: Size-dependent electron–hole exchange interaction in Si nanocrystals. Appl Phys Lett 2000, 76: 351. 10.1063/1.125751View Article
- Priolo F, Franzo G, Coffa S, Carnera A: Excitation and nonradiative deexcitation processes of Er3+ in crystalline Si. Phys Rev B 1998, 57: 4443. 10.1103/PhysRevB.57.4443View Article
- Delerue C, Allan G, Lannoo M: Optical band gap of Si nanoclusters. J Lum 1999, 80: 65.View Article
- Imakita K, Fujii M, Yamaguchi Y, Hayashi S: Interaction between Er ions and shallow impurities in Si nanocrystals within SiO2. Phys Rev B 2005, 71: 115440.View Article
- Comedi D, Zalloum OHY, Irving EA, Wojcik J, Roschuk T, Flynn MJ, Mascher P: X-ray-diffraction study of crystalline Si nanocluster formation in annealed silicon-rich silicon oxides. J Appl Phys 2006, 99: 023518. 10.1063/1.2162989View Article
- Heng CL, Zalloum OHY, Wojcik J, Roschuk T, Mascher P: On the effects of double-step anneal treatments on light emission from Er-doped Si-rich silicon oxide. J Appl Phys 2008, 103: 024309. 10.1063/1.2829809View Article
- Podhorodecki A, Zatryb G, Misiewicz J, Wojcik J, Mascher P: Influence of the annealing temperature and silicon concentration on the absorption and emission properties of Si nanocrystals. J Appl Phys 2007, 102: 043104. 10.1063/1.2772501View Article
- Podhorodecki A, Misiewicz J, Gourbilleau F, Rizk R: Absorption mechanisms of silicon nanocrystals obtained at different hydrogen partial pressure in co-sputtered (SRSO) film. Electrochemical Solid State Lett. 2008, 11: K31-K33. 10.1149/1.2828207View Article
- Hao XJ, Podhorodecki A, Shen YS, Zatryb G, Misiewicz J, Green MA: Effects of non-stoichiometry of O/Si ratio on the structural and optical properties of silicon quantum dots in a silicon dioxide matrix. Nanotechnology 2009, 20: 485703. 10.1088/0957-4484/20/48/485703View Article
- Pacchioni G, Skuja L, Griscom DL: Defects in SiO2 and Related Dielectrics: Science and Technology. New York: Springer; 2000:73.View Article
- Zatsepin AF, Biryukov DY, Kortov VS: Analysis of OSEE spectra of irradiated dielectrics. Latv J Phys Tech Sci 2000, 6: 83.
- Skuja L, Güttler B, Schiel D, Silin AR: Quantitative analysis of the concentration of interstitial O2 molecules in SiO2 glass using luminescence and Raman spectroscopy. J Appl Phys 1998, 83: 6106. 10.1063/1.367480View Article
- Cueff S, Labbé C, Dierre B, Fabbri F, Sekiguchi T, Portier X, Rizk R: Investigation of emitting centers in SiO2 codoped with silicon nanoclusters and Er3+ ions by cathodoluminescence technique. J Appl Phys 2010, 108: 113504. 10.1063/1.3517091View Article
- Barfels T: Kathodolumineszenz amorpher und kristalliner Modifikationen von SiO2 und GeO2. PhD dissertation: Rostock University; 2001.
- Varshni VP: Temperature dependence of the energy gap in semiconductors. Physica 1967, 34: 149. 10.1016/0031-8914(67)90062-6View Article
- Cho Y, Gainer GH, Fischer HJ, Song JJ, Keller S, Mishra UK, DenBaars SP: S-shaped temperature-dependent emission shift and carrier dynamics in InGaN/GaN multiple quantum wells. Appl Phys Lett 1998, 73: 1370. 10.1063/1.122164View Article
- Street RA: Hydrogenated Amorphous Silicon. Cambridge: Cambridge University Press; 2005. Chap. 7 Chap. 7
- Zatryb G, Podhorodecki A, Hao XJ, Misiewicz J, Shen YS, Green MA: Correlation between stress and carriers nonradiative recombination for silicon nanocrystals in an oxide matrix. Nanotechnology 2011, 22: 335703. 10.1088/0957-4484/22/33/335703View Article
- Polman A: Erbium implanted thin film photonic materials. J Appl Phys 1997, 82: 1. 10.1063/1.366265View Article
- Przybyliska H, Jantsch W, Suprun-Belevitch Y, Stephikova M, Palmetshofer L, Hendorfer G, Kozanecki A, Wilson RJ, Sealy BJ: Optically active erbium centers in silicon. Phys Rev B 1996, 54: 2532. 10.1103/PhysRevB.54.2532View Article
- Heitmann J, Schmidt M, Zacharias M, Timoshenko VY, Lisachenko MG, Kashkarov PK: Fabrication and photoluminescence properties of erbium doped size-controlled silicon nanocrystals. Materials Science and Engineering B 2003, 105: 214–220. 10.1016/j.mseb.2003.08.048View Article
- Falconieri M, Borsella E, Enrichi F, Franzo G, Priolo F, Iacona F, Gourbilleau F, Rizk R: Time dependence and excitation spectra of the photoluminescence emission at 1.54lm in Si-nanocluster and Er co-doped silica. Opt Mater 2005, 27: 884–889. 10.1016/j.optmat.2004.08.029View Article
- Falconieri M, Borsella E, De Dominicis L, Enrichi F, Franzò G, Priolo F, Iacona F, Gourbilleau F, Rizk R: Probe of the Si nanoclusters to Er3+ energy transfer dynamics by double-pulse excitation. Appl Phys Lett 2005, 87: 061109. 10.1063/1.2001753View Article
- Watanabe K, Fuji M, Hayashi S: Resonant excitation of Er3+ by the energy transfer from Si nanocrystals. J Appl Phys 2001, 90: 4761. 10.1063/1.1409572View Article
- Kuritsyn D, Kozanecki A, Przybylinska H, Jantsch W: Defect-mediated and resonant optical excitation of Er3+ ions in silicon-rich silicon oxide. Appl Phys Lett 2003, 83: 4160. 10.1063/1.1627483View Article
- Gschneidner KA: Handbook of the Physics and Chemistry of Rare Earths. Philadelphia: Elsevier; 1998:25.
- Podhorodecki A, Zatryb G, Misiewicz J, Gourbilleau F, Dufour C: Temperature dependent emission quenching in silicon-rich oxide films. J Nanoscience and Nanotechnology 2010, 10: 1. 10.1166/jnn.2010.1484View Article
- Saeed S, Timmerman D, Gregorkiewicz T: Dynamics and microscopic origin of fast 1.5 μm emission in Er-doped SiO2 sensitized with Si nanocrystals. Phys Rev B 2011, 83: 155323.View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.